lecture notes

```

Torsion Testing
o What is a torsion test?
 Torsion tests apply a load to a specimen by twisting the ends of the
specimen in opposite directions
o Why perform a torsion test?
 Get several values similar to those from a tension test
 Values obtained include:
 Modulus of Rigidity
o Sometimes called the Shear Modulus
o Similar to Modulus of Elasticity for tension test
 Shearing Yield Point
 Ultimate Shear Strength
 Maximum Elastic Torque
 Fully Plastic Torque
Lab Procedure
o We will split into two large groups to perform the tests
 One large group will work with me on one machine
 Other large group will work with TA on other machine
 Each group needs to collect their own data
 For Example: Group 1, 2, and 3 each have their own data sheet
even though the data will be identical between groups
o An A36 steel bar will be used in the tests
o Equipment used
TorsionAssignmentTorsion Testing Equipment
o Measurements
 Diameter of the rod before testing
 This needs to be from the center of the bar to the tip of the pointer
 Easiest to find by measuring from the outside of the bar to the
o One end of the bar will remain fixed while the other end is slowly twisted by
applying torque
 You will collect data at each 100 in-lb increment of torque from 0 to 1000
in-lb of torque
 Once the torque is above 1000 in-lb you will take readings at every 0.1 in
increment of arc length
 Continue these readings until the fully plastic torque has been
clearly reached
o Fully plastic torque occurs when the bar continues to twist
but the amount of torque required remains constant
 It is up to the groups to decide when enough data points have been
collected
o Want several data points in the fully plastic region to
ensure good results
 After fully plastic torque has been established you will no longer need to
collect data at regular intervals
 We will continue to twist the bar until it fractures


Only thing left to find will be the maximum torque
Torque vs. Angle of Twist Diagram
o These are the values you will actually be recording in the lab
o Show how to determine the Fully Plastic Torque and the Maximum Elastic
Torque
o Draw figure on board

o Formulas


s

Linear
Elastic
Portion
rtrop
TL

JG
 T   L 
G
 
    J 


 J  d 4  c 4 (polar moment of inertia for circular cross section)
32
2
 TFP read from data and graph
3
 TE  TFP
4
Shearing Stress-Strain Diagram
o Element on the surface of the bar oriented along the axis
 Has only shear stresses acting on it (pure shear)
 Draw figure on board


o Similar to tension stress-strain diagrams
 Normal Stress is replaced by Shear Stress
 Normal Strain is replace by Shear Strain
 Assumes a linear elastic, perfectly plastic material
 Draw figure on board
τy
G
o Formulas





Tc
J
c

L

(applies only in linear elastic portion)
G

T c
y  E
J
 
Yielding in Circular Shafts
TorsionShort Version

o Yielding starts at outer surface since maximum stresses are present there
o As material yields there is a plastic shell that forms on the outside of the material
o Eventually the entire cross section will yield and the fully plastic state will be
reached
Fracture Surfaces
o Ductile Materials
 Fail due to shear stress
 Fracture surface should be oriented with shear stresses on element
 Results in a 90º fracture surface
TorsionFracture Geometry
o Brittle Materials
 Fail due to normal stresses
 Remember that an element oriented 45º from a pure shear element has
only normal stresses
 Results in brittle materials fracturing with a 45º fracture surface
o The fracture surfaces are oriented just the opposite of what we found in the
tension tests

Direct Shear Test
o While we are waiting on the torsion testing specimen to fracture we will perform
a direct shear test
o Will work as an entire section
o Material to test will be an A36 bar identical to the one used for torsion testing
o Procedure
 Measure the diameter of the A36 steel bar
 Load specimen in the shear testing fixture
 Apply load to the specimen using a cross-head speed of 0.1 in/min
 Run the test until the computer stops the cross-head
 Record the 0.2% offset yield load from the computer
 Record the maximum load from the computer
o Calculations
 Find the shearing yield strength by applying
V
Vy
 S sy  y 
A    2 
 2 4 d 

 
 Find the ultimate shearing strength using
V
Vmax
 Sus  max 
A
   2 
 2 4 d 

 

Assignment
o Memo worth 100 points
 Attach your initialed original data sheet
 Experimental Results
 Torsion Testing
o Create a plot of torque (T) vs. angle of twist(φ) using your
data
o Based on your data and plot

Determine the Fully Plastic Torque (TFP)

Calculate the Maximum Elastic Torque (TE)
o Use linear regression to calculate the slope of the linear
elastic portion of the plot

Only use data points up to the Maximum Elastic
Torque
o Use your slope to calculate the modulus of rigidity (G)
o Calculate the shearing yield strength and ultimate shearing
strength
 Direct Shear Testing
o Calculate and report the shearing yield strength
o Calculate and report the ultimate shearing strength
 Discussion of Results
 Discuss how well your data points fit the linear regression line
 Compare your shearing yield strength and ultimate shearing
strength between the torsion test and the direct shear test


Look up a reference value for G and compare your experimental
value to the reference value
Presentation
o Each group will come to the board and fill in the following values
TE (in-lb)
TFP (in-lb)
Experimental G (ksi)
Experimental  y (ksi)
o Two random groups will be selected to answer questions about the lab
```
Related flashcards
Curves

20 Cards

Analytic geometry

14 Cards

Tensors

20 Cards